Download presentation

Presentation is loading. Please wait.

1
**Chapter 3: The Structure of Crystalline Solids**

ISSUES TO ADDRESS... • How do atoms assemble into solid structures? • How does the density of a material depend on its structure? • When do material properties vary with the sample (i.e., part) orientation?

2
**Energy and Packing • Non dense, random packing**

typical neighbor bond length bond energy • Dense, ordered packing Energy r typical neighbor bond length bond energy Dense, ordered packed structures tend to have lower energies.

3
**Materials and Packing Si Oxygen Crystalline materials...**

• atoms pack in periodic, 3D arrays • typical of: -metals -many ceramics -some polymers crystalline SiO2 Adapted from Fig. 3.23(a), Callister & Rethwisch 8e. Si Oxygen Noncrystalline materials... • atoms have no periodic packing • occurs for: -complex structures -rapid cooling "Amorphous" = Noncrystalline noncrystalline SiO2 Adapted from Fig. 3.23(b), Callister & Rethwisch 8e.

4
** Metallic Crystal Structures**

How can we stack metal atoms to minimize empty space? 2-dimensions vs. Now stack these 2-D layers to make 3-D structures

5
**Metallic Crystal Structures**

• Tend to be densely packed. • Reasons for dense packing: - Typically, only one element is present, so all atomic radii are the same. - Metallic bonding is not directional. - Nearest neighbor distances tend to be small in order to lower bond energy. - Electron cloud shields cores from each other • Have the simplest crystal structures. We will examine three such structures...

6
**Simple Cubic Structure (SC)**

• Rare due to low packing density (only Po has this structure) • Close-packed directions are cube edges. • Coordination # = 6 (# nearest neighbors) Click once on image to start animation (Courtesy P.M. Anderson)

7
**Atomic Packing Factor (APF)**

Volume of atoms in unit cell* APF = Volume of unit cell *assume hard spheres • APF for a simple cubic structure = 0.52 Adapted from Fig. 3.24, Callister & Rethwisch 8e. close-packed directions a R=0.5a contains 8 x 1/8 = 1 atom/unit cell atom volume atoms unit cell 4 3 p (0.5a) 1 APF = 3 a unit cell volume

8
**Body Centered Cubic Structure (BCC)**

• Atoms touch each other along cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. ex: Cr, W, Fe (), Tantalum, Molybdenum • Coordination # = 8 Adapted from Fig. 3.2, Callister & Rethwisch 8e. Click once on image to start animation (Courtesy P.M. Anderson) 2 atoms/unit cell: 1 center + 8 corners x 1/8

9
**Atomic Packing Factor: BCC**

• APF for a body-centered cubic structure = 0.68 a R a 3 a a 2 length = 4R = Close-packed directions: 3 a Adapted from Fig. 3.2(a), Callister & Rethwisch 8e. APF = 4 3 p ( a/4 ) 2 atoms unit cell atom volume a

10
**Face Centered Cubic Structure (FCC)**

• Atoms touch each other along face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. ex: Al, Cu, Au, Pb, Ni, Pt, Ag • Coordination # = 12 Adapted from Fig. 3.1, Callister & Rethwisch 8e. Click once on image to start animation 4 atoms/unit cell: 6 face x 1/2 + 8 corners x 1/8 (Courtesy P.M. Anderson)

11
**Atomic Packing Factor: FCC**

• APF for a face-centered cubic structure = 0.74 a 2 a maximum achievable APF Close-packed directions: length = 4R = 2 a Unit cell contains: 6 x 1/2 + 8 x 1/8 = 4 atoms/unit cell Adapted from Fig. 3.1(a), Callister & Rethwisch 8e. APF = 4 3 p ( 2 a/4 ) atoms unit cell atom volume a

12
**FCC Stacking Sequence • ABCABC... Stacking Sequence • 2D Projection**

A sites B C sites A B sites C A C A A B C • FCC Unit Cell

13
**Hexagonal Close-Packed Structure (HCP)**

• ABAB... Stacking Sequence • 3D Projection • 2D Projection c a A sites B sites Bottom layer Middle layer Top layer Adapted from Fig. 3.3(a), Callister & Rethwisch 8e. • Coordination # = 12 6 atoms/unit cell • APF = 0.74 ex: Cd, Mg, Ti, Zn • c/a = 1.633

14
**Theoretical Density, r Density = = n A = VC NA**

Cell Unit of Volume Total in Atoms Mass Density = = VC NA n A = where n = number of atoms/unit cell A = atomic weight VC = Volume of unit cell = a3 for cubic NA = Avogadro’s number = x 1023 atoms/mol

15
**Theoretical Density, r = a R Ex: Cr (BCC) A = 52.00 g/mol**

R = nm n = 2 atoms/unit cell a = 4R/ 3 = nm Adapted from Fig. 3.2(a), Callister & Rethwisch 8e. = a3 52.00 2 atoms unit cell mol g volume 6.022 x 1023 theoretical = 7.18 g/cm3 ractual = 7.19 g/cm3

16
**Densities of Material Classes**

In general Graphite/ r metals r ceramics r polymers Metals/ Composites/ > > Ceramics/ Polymers Alloys fibers Semicond 30 Why? B ased on data in Table B1, Callister Metals have... • close-packing (metallic bonding) • often large atomic masses 2 Magnesium Aluminum Steels Titanium Cu,Ni Tin, Zinc Silver, Mo Tantalum Gold, W Platinum *GFRE, CFRE, & AFRE are Glass, Carbon, & Aramid Fiber-Reinforced Epoxy composites (values based on 60% volume fraction of aligned fibers 10 in an epoxy matrix). G raphite Silicon Glass - soda Concrete Si nitride Diamond Al oxide Zirconia Ceramics have... • less dense packing • often lighter elements 5 3 4 (g/cm ) 3 Wood AFRE * CFRE GFRE* Glass fibers Carbon fibers A ramid fibers H DPE, PS PP, LDPE PC PTFE PET PVC Silicone Polymers have... • low packing density (often amorphous) • lighter elements (C,H,O) r 2 1 Composites have... • intermediate values 0.5 0.4 0.3 Data from Table B.1, Callister & Rethwisch, 8e.

17
**Crystals as Building Blocks**

• Some engineering applications require single crystals: -- diamond single crystals for abrasives -- turbine blades Fig. 8.33(c), Callister & Rethwisch 8e. (Fig. 8.33(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) • Properties of crystalline materials often related to crystal structure. -- Ex: Quartz fractures more easily along some crystal planes than others. (Courtesy P.M. Anderson)

18
**Polycrystals Anisotropic**

• Most engineering materials are polycrystals. Adapted from Fig. K, color inset pages of Callister 5e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) 1 mm Isotropic • Nb-Hf-W plate with an electron beam weld. • Each "grain" is a single crystal. • If grains are randomly oriented, overall component properties are not directional. • Grain sizes typically range from 1 nm to 2 cm (i.e., from a few to millions of atomic layers).

19
**Single vs Polycrystals**

E (diagonal) = 273 GPa E (edge) = 125 GPa • Single Crystals -Properties vary with direction: anisotropic. Data from Table 3.3, Callister & Rethwisch 8e. (Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) -Example: the modulus of elasticity (E) in BCC iron: • Polycrystals -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (Epoly iron = 210 GPa) -If grains are textured, anisotropic. 200 mm Adapted from Fig. 4.14(b), Callister & Rethwisch 8e. (Fig. 4.14(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].)

20
Polymorphism Two or more distinct crystal structures for the same material (allotropy/polymorphism) titanium , -Ti carbon diamond, graphite BCC FCC 1538ºC 1394ºC 912ºC -Fe -Fe -Fe liquid iron system

21
Crystal Systems Unit cell: smallest repetitive volume which contains the complete lattice pattern of a crystal. Fig. 3.4, Callister & Rethwisch 8e. 7 crystal systems 14 crystal lattices a, b, and c are the lattice constants

22
**Point Coordinates z Point coordinates for unit cell center are c**

x y a b c 000 111 Point coordinates for unit cell center are a/2, b/2, c/ ½ ½ ½ Point coordinates for unit cell corner are 111 Translation: integer multiple of lattice constants identical position in another unit cell z 2c y b b

23
**Crystallographic Directions**

z pt. 2 head Example 2: pt. 1 x1 = a, y1 = b/2, z1 = 0 pt. 2 x2 = -a, y2 = b, z2 = c y pt. 1: tail x => -2, 1/2, 1 Multiplying by 2 to eliminate the fraction -4, 1, 2 where the overbar represents a negative index [ 412 ] => families of directions <uvw>

24
**Crystallographic Directions**

z Algorithm 1. Vector repositioned (if necessary) to pass through origin. 2. Read off projections in terms of unit cell dimensions a, b, and c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvw] y x ex: 1, 0, ½ Lecture 2 ended here => 2, 0, 1 => [ 201 ] -1, 1, 1 where overbar represents a negative index [ 111 ] => families of directions <uvw>

25
**Linear Density 3.5 nm a 2 LD = Linear Density of Atoms LD = [110]**

Number of atoms Unit length of direction vector a [110] ex: linear density of Al in [110] direction a = nm # atoms length 1 3.5 nm a 2 LD - = Adapted from Fig. 3.1(a), Callister & Rethwisch 8e.

26
**HCP Crystallographic Directions**

- a3 a1 a2 z Algorithm 1. Vector repositioned (if necessary) to pass through origin. 2. Read off projections in terms of unit cell dimensions a1, a2, a3, or c 3. Adjust to smallest integer values 4. Enclose in square brackets, no commas [uvtw] dashed red lines indicate projections onto a1 and a2 axes a1 a2 a3 -a3 2 a 1 Adapted from Fig. 3.8(a), Callister & Rethwisch 8e. [ 1120 ] ex: ½, ½, -1, =>

27
**HCP Crystallographic Directions**

Hexagonal Crystals 4 parameter Miller-Bravais lattice coordinates are related to the direction indices (i.e., u'v'w') as follows. Fig. 3.8(a), Callister & Rethwisch 8e. - a3 a1 a2 z = ' w t v u ) ( + - 2 3 1 ] uvtw [

28
**Crystallographic Planes**

Adapted from Fig. 3.10, Callister & Rethwisch 8e.

29
**Crystallographic Planes**

Miller Indices: Reciprocals of the (three) axial intercepts for a plane, cleared of fractions & common multiples. All parallel planes have same Miller indices. Algorithm 1. Read off intercepts of plane with axes in terms of a, b, c 2. Take reciprocals of intercepts 3. Reduce to smallest integer values 4. Enclose in parentheses, no commas i.e., (hkl)

30
**Crystallographic Planes**

z x y a b c example a b c Intercepts Reciprocals 1/ / / Reduction Miller Indices (110) example a b c z x y a b c Intercepts 1/ Reciprocals 1/½ 1/ 1/ Reduction Miller Indices (100)

31
**Crystallographic Planes**

z x y a b c example a b c Intercepts 1/ /4 Reciprocals 1/½ 1/ /¾ /3 Reduction Miller Indices (634) (001) (010), Family of Planes {hkl} (100), (001), Ex: {100} = (100),

32
**Crystallographic Planes (HCP)**

In hexagonal unit cells the same idea is used a2 a3 a1 z example a a a c Intercepts -1 1 Reciprocals / -1 1 Reduction -1 1 Miller-Bravais Indices (1011) Adapted from Fig. 3.8(b), Callister & Rethwisch 8e.

33
**Crystallographic Planes**

We want to examine the atomic packing of crystallographic planes Iron foil can be used as a catalyst. The atomic packing of the exposed planes is important. Draw (100) and (111) crystallographic planes for Fe. b) Calculate the planar density for each of these planes.

34
**Virtual Materials Science & Engineering (VMSE)**

• VMSE is a tool to visualize materials science topics such as crystallography and polymer structures in three dimensions • Available in Student Companion Site at and in WileyPLUS

35
**VMSE: Metallic Crystal Structures & Crystallography Module**

• VMSE allows you to view crystal structures, directions, planes, etc. and manipulate them in three dimensions

36
**Unit Cells for Metals FCC Structure HCP Structure**

• VMSE allows you to view the unit cells and manipulate them in three dimensions • Below are examples of actual VMSE screen shots FCC Structure HCP Structure

37
**VMSE: Crystallographic Planes Exercises**

Additional practice on indexing crystallographic planes

38
**Planar Density of (100) Iron**

Solution: At T < 912ºC iron has the BCC structure. 2D repeat unit R 3 4 a = (100) Radius of iron R = nm Adapted from Fig. 3.2(c), Callister & Rethwisch 8e. = Planar Density = a 2 1 atoms 2D repeat unit nm2 12.1 m2 = 1.2 x 1019 R 3 4 area

39
**Planar Density of (111) Iron**

Solution (cont): (111) plane 1 atom in plane/ unit surface cell 2 a atoms in plane atoms above plane atoms below plane 2D repeat unit 3 h = a 2 3 2 R 16 4 a ah area = ø ö ç è æ 1 = nm2 atoms 7.0 m2 0.70 x 1019 3 2 R 16 Planar Density = 2D repeat unit area

40
**VMSE Planar Atomic Arrangements**

• VMSE allows you to view planar arrangements and rotate them in 3 dimensions BCC (110) Plane

41
X-Ray Diffraction Diffraction gratings must have spacings comparable to the wavelength of diffracted radiation. Can’t resolve spacings Spacing is the distance between parallel planes of atoms.

42
**X-Rays to Determine Crystal Structure**

• Incoming X-rays diffract from crystal planes. Adapted from Fig. 3.20, Callister & Rethwisch 8e. reflections must be in phase for a detectable signal spacing between planes d incoming X-rays outgoing X-rays detector q l extra distance travelled by wave “2” “1” “2” X-ray intensity (from detector) q c d = n l 2 sin Measurement of critical angle, qc, allows computation of planar spacing, d.

43
**X-Ray Diffraction Pattern**

z x y a b c z x y a b c z x y a b c (110) (211) Intensity (relative) (200) Diffraction angle 2q Diffraction pattern for polycrystalline a-iron (BCC) Adapted from Fig. 3.22, Callister 8e.

44
**SUMMARY • Atoms may assemble into crystalline or amorphous structures.**

• Common metallic crystal structures are FCC, BCC, and HCP. Coordination number and atomic packing factor are the same for both FCC and HCP crystal structures. • We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). • Crystallographic points, directions and planes are specified in terms of indexing schemes. Crystallographic directions and planes are related to atomic linear densities and planar densities.

45
**SUMMARY • Materials can be single crystals or polycrystalline.**

Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains. • Some materials can have more than one crystal structure. This is referred to as polymorphism (or allotropy). • X-ray diffraction is used for crystal structure and interplanar spacing determinations.

46
ANNOUNCEMENTS Reading: Core Problems: Self-help Problems:

Similar presentations

OK

ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties.

ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on weapons of mass destruction book Ppt on eye oswego Ppt on power line carrier communications Broken text ppt on file Ppt on diodes and transistors Ppt on computer software download Ppt on icici prudential life insurance Short ppt on social networking sites Ppt on amplitude shift keying modem Ppt on bio battery free download